MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS


 Arnold Lee
 1 years ago
 Views:
Transcription
1 MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France SUMMARY The present paper deals with a computational strategy to model the strength of bolted joints in composite structures. The rupture of the global structure is determined thanks a twolevel level strategy. At the local scale, a detailed Finite Element model of the singlebolt joint, taking into account delamination, is used. Keywords: bolted joints, bearing failure, progressive damage, nonlocal calculation methods, multilevel strategy INTRODUCTION Due to their high specific strength and stiffness, Carbon FibreReinforced Plastics (CFRP) are increasingly used in aeronautical applications. These applications usually require the use of mechanical joints in order to transfer loads between composite laminates and other composite or metallic parts. Therefore, ability to joint elements efficiently is necessary for a full exploitation of high performance fibrereinforced plastics. Nevertheless, ensuring the load transfers between composite and other composite or metallic parts remains problematic. Since the use of bonded joints is often prohibited by the industrial imperatives of reproducibility and maintenance, mechanically fastened joints  such as bolted or riveted joints  are preferentially used. However, composite components are considerably weakened by the drilling of holes, mostly because of the resulting high stress concentrations. For instance, the strength of a bolted joint could be, in some cases, 50% lower as compared with a plane plate. The mechanical joint is often a limiting factor for the overall performance of the structure that severely handicaps the replacement of the existing light alloy structures by composite solutions. It is thus an absolute necessity to predict the behaviour and the strength of bolted joints. Two kinds of approaches are proposed in the literature to attain this goal. The first one, could be called brittle criterion approach. The main idea consists in using, as a postprocessing of an elastic finite element calculation, a failure criterion using stresses calculated on characteristic curves associated to each mode of rupture [ 1 ]. However, the characteristic lengths involved in these methods are a function of the stacking sequence, of the geometry of the joints etc... This is the reason why some authors have proposed a second kind of approach that could be called "progressive damage model". The main idea of this approach consists in taking into account the effect of the most significant physical phenomena experimentally observed : nonlinear behaviour of the matrix, matrix rupture, fibre rupture and delamination. Lot of authors have focused on the matrix and fibre ruptures (see [ 3, 4]) since these two modes of ruptures are responsible of the final failure in shear (matrix failure), in tensile (fibre failure in tension) and bearing (fibre failure in compression). The delamination, which has an
2 important effect on the global behaviour and the final rupture, is most of the time studied using rupture criterion and its effect is taken into account by few authors [ 5]. Moreover, using complex softening models lead to numerical problems [ 6] that are not always adressed. The definition of the final failure, which is another very important point, is generally characterized by the divergence of the FE calculation. This article aims at proposing a strategy adapted to complex fastened composite joints. The first section of this paper is thus devoted to the presentation of a 3D progressive failure approach. A cohesive zone model is used in order to describe the delamination and its effect. A comparison with experimental results is also proposed. The second section is devoted to the application of this approach to an industrial case thanks to the use of virtual testing. Finally, a conclusion and a discussion are proposed in the last section. MULTISCALE ANALYSIS OF SINGLEBOLT COMPOSITE JOINTS Presentation of the multiscale model to describe the behaviour and the rupture of bolted joints The proposed approach is based on the physical phenomena observed in composite joints (matrix crack, fibre failure in tension and in compression, delamination). The ply level has been considered as the pertinent scale to describe these phenomena. The behaviour of the unidirectional ply is based on a damage thermoviscoelastic model and is written as follows : C ~ ve th σ = : ( ε ε ε ) where σ is the stress, C ~ th is the elastic stiffness tensor, ε is the total strain, ε is the ve thermal strain and ε the viscoelastic strain (modelled using a viscoelastic spectral model [ 7]). The mesoscopic failure criterion is based on physical principles and makes a distinction between the fibre failure (FF, criterion f 1 ) and the matrix failure (IFF, criterion f ) modes. f ε 1 ε 1 f 1 = X t X c ε ε = Yt Yc ε S 6 c with X X = X, = X, if X 0, X if X 0, X = 0, = 0, if X < 0 if X > 0 The effect of a crack on the mechanical properties of a ply is described thanks to a damage model. After the first failure of a ply in the laminate (failure criterion value is higher than 1), the effective elastic compliance S ~ of the failed ply is increased ~ FF d f = α 1 S = S d1h1 d H d& i 0 IFF d = β f 1 0 where S is the initial elastic compliance, H 1 and H are forth order tensors that respectively represent the effect of fiber failure (damage variable d 1 ) and interfibre
3 failure (damage variable d 1 ). The identification of this model necessitates only five tests performed on a UD ply and one test on a laminate to identify the parameter β. In order to avoid numerical problems of damage localization due to the use of softening degradation rules, a delayed damage approach is employed [ 8]. The indetification of the parameter of this approach does not necessitate any test and could be seen as a numerical parameter. Cohesive zone elements are used to simulate the interface between the plies. The behaviour of these interfaces is elastic with softening damage rules in normal tension and shear; moreover, friction is taken into account in shear. The mechanical behavior of the interface is described by the relation between the normal and tangential relative displacements (Un, Ut) of the nodes, and their respective normal and tangential tractions (Tn, Tt). The damage evolution is taken into account by the damage variable λ which combines the tension and the shear damages as follows [ 9]: λ = U δ n n U t δ t The nonlinear relations between ( U, U ) and ( T, T n t n t ) have the form: U n Tn = F( λ) δ n U t Tt = α F( λ) δ t 7 and F(λ) is chosen as F( λ ) = σ max (1 λ) for 0 λ 1, where σ max and ασ max are 4 respectively the maximum values of T n and T t in pure modes. The damage parameter λ varies continuously from 0 (locally bonded case) to 1 (locally debonded case). The complete separation between two corresponding nodes occurs for λ=1 (F(λ)=0) so that δ n and δ t are the maximum values of the relative displacements U n and U t in pure normal and pure shear modes respectively. The interfacial parameters have been identified thanks to classical fracture mechanics tests. Finite Element multimodel strategy A mesh convergence study has been performed in [ 10]. This study has shown that it is possible to establish some rules which permit to insure that the mesh is fine enough. Moreover, in order to model the inply damage and the delamination, it is necessary to describe the laminate thanks (at least) one element by ply and cohesive zone elements between each plies. Finally, the number of degree of freedom could become tremendous when the number of plies increase. In order to overcome these difficulties a multimodel strategy is used. The main idea consists in reducing the complexity of the models (FE mesh and material behavior) as a function of the distance of the hole (see Figure 1. The parts located far from the zone of interest are modeled using only one element in the thickness and the homogenized orthotropic elastic behavior of the laminate. The transition with the zone of interest is performed using multilayer element and the elastic behavior for each ply.
4 Finally, in the zone of interest, at least one element in the thickness of a ply is used and a cohesive zone element is introduced between the plies. In this zone, the behaviour of the ply is described using the proposed model. In order to decrease the number of dof, the cohesive zone elements are only introduced near the singularities. The junction between each parts of the mesh is insured thanks to displacement conditions between the nodes (Multiple Point Constraints). Zone of interest Volume element elastic laminate behaviour Volume element Nonlinear ply behaviour CZM Multilayer element elastic ply behaviour Volume element CZM Nonlinear ply behaviour Figure 1 : Multimodel strategy The mains difficulties of this approach lies in the choice of the size of the zone of interest. Indeed, if the damage (ply rupture of delamination) reach the border of the interest zone the modeling has no more physical sense. However, a progressive meshing strategy is under development to overcome this difficulty. It is worth to mention that in the present study, a great attention has been paid to this problem. Comparison with experimental results The present section is devoted to the comparison with experimental results. A progressive comparison is proposed. The first comparisons are performed on T300/914 laminates [ 10]. First of all, test cases on open hole and filled hole plates are investigated. The next step concerns the modeling of bearing tests with different diameter of hole. Finally, tests on double lap joints subjected to tesile loads and bypass and bearing loadings are investigated. The last comparison concerns the same kind of tests but performed on another material (T700/M1 material). The parameters of the model have been identify thanks to experimental tests performed on UD ply provided in [ 10]. Moreover, it is well known that the coefficient of friction between the insert and the composite is a very sensitive parameters. As suggested in [ 11], this coefficient has been chosen equal to Openhole and filledhole tests on T300/914 laminate. The experimental and numerical results are presented in Table 1 and in figures 1 and. All these results has been obtained on a [90 /0 /90 /0 ] s laminate. The thickness is close
5 to mm, the diameter of the hole (d) is equal to 6 mm and the ration width (w) over diameter is equal to 3. Each test has been repeated twice. The first ply failure loading has been measured thanks to acoustic emission. Table 1 : Comparison between experimental and numerical results for openhole and filledhole test specimens First ply failure (N) Final failure (N) Type of specimen Test Test Model Error Model Error (mean value) (mean value) Openhole % % Filledhole % % Load (N) (a) Displacement (mm) Figure : Comparison between experimental and numerical results for openhole tests (b) (c) Figure 3 : Pattern of damage (a) delamination, (b) fibre ruptures and (c) matrix ruptures at the end of the test The results obtained by the model are in quite good agreement with the experimental results as well as at a global point of view (loading curve, final failure) and as a local one (first ply failure). It could be noted that, due to the use of a delayed damage approach to overcome localization, the final failure is slightly overestimate. Bearing tests on T300/914 laminate. The experimental and numerical results are presented in Table. The staking sequence and the geometry are the same than in the previous paragraph. Different diameters of hole have been investigated. For each diameter the ratio w/d is equal to 3. The comparison shows that the model permits to reproduce in a quite good manner the evolution of the bearing strength as a function of the diameter of the hole.
6 Table : Comparison between experimental and numerical results for bearing tests First ply failure (MPa) Rupture en matage (MPa) d Test (mm) Tests Model (mean Error Model Error (mean value) value) % % % % % % % % Bypass and bearing loading tests on double lap joint T300/914 laminate. The experimental geometry is presented in Table 3. First, a bearing load equal to 500 N is applied to the test specimen. A tensile load is then applied up to the rupture. The first test is performed on a 3 plies specimen with the [(45/0/45/90) 4 ] s stacking sequence. The second test is performed on the same kind of specimen only disoriented of.5. Table 3 : Comparison between experimental and numerical results for bypass and bearing tests Failure load (N) Test D w e L (mm) (mm) (mm) (mm) Model Test Error 1 6, % 6, % The experimental failure occurs by traction. The modelings confirm this scenario and show that there is no bearing crack initiated prior to the rupture. Figure 4 shows the fibre rupture located at 90 of the load axis and the delamination pattern. The numerical results are in quite good agreement with the experimental ones. It seems that the model underestimates the failure load. It could be explained by the lack of knowledge (i) in the longitudinal compressive strength and (ii) in the kinetic of this mode of failure.
7 Figure 4 : In the left: interfacial delamination between ply at 45 and 0. In the right: fibre failure in 0 plies. Bearing test and openhole tests on T700/M1 laminates In order to validate the present model on an other material (T700/M1 with a ply thickness equal to 0.6mm), tensile tests on openhole laminate and a bearing test have been realized [ 1]. The openhole tensile tests have been performed on a 3 plies laminate ([0/45/90/45/90/45/90/45/90/45/0/45/90] s ). The width of the plate is equal to 45.7mm and three different diameters of hole have been investigated (see Table 4). The bearing test has been performed on a [90/45/0 /45/0 /45/0/45/0 /45/90/45/0] s test specimen (the geometry is given by w=49.6mm, d=9.5mm and e=3.8mm, see table 3). Table 4 : Comparison between experimental and numerical results of openhole tests and bearing test on T700/M1 laminates d Open hole specimens Bearing specimens (mm) Test (kn) Model (kn) Error Test (kn) Model (kn) Error 7, % 9, % % 1, % The numerical results are in quite good agreement with the experimental ones. As for the T300/914 laminates, it seems that the model (i) overestimates the experimental results for the open hole tests specimens and (ii) underestimates the experimental results for bearing tests. MULTILEVEL ANALYSIS OF COMPLEX INDUSTRIAL COMPOSITE JUNCTIONS Industrial approach for complex industrial composite joints In an industrial point of view, a twolevel strategy is used in order to describe the rupture of complex bolted joints in composite structure involving several hundred of fixations (see fig., left of the figure). Firstly, global calculation is performed in order to evaluate the behavior of the whole junction in its environment. Because of the geometrical complexity of the structure, coarse meshes and simple material behavior are used. The joints are replaced by springs with an equivalent stiffness identified according
8 a semiempirical formula provided. Secondly, strength of the critical fixations is evaluated at locallevel calculations. The loads issued from the global calculation are injected as input data for the local reanalysis of the critical fasteners, using semiempirical models (see Figure 5). It is supposed that there is no bolthole clearance. By respecting some classical design guidelines for the geometry of the joint and the choice of the stacking sequence, shearout failure mode can be easily avoided. Therefore the critical failure mode taken into account in the model is a combination of tensile and bearing failure modes. Failure occurs when the following criterion is reached : Where: K t n ( σ t K m. σ m ) σ r. (3) σ t n is the average tensile stress in the net crosssection, σ m is the average bearing stress, σ r is the admissible stress, K t and K m are respectively the hole coefficient and the bearing coefficient. K t and K m are empirical coefficients whose identification requires many experiments. These coefficients depend on the material, the stacking sequence, the nature of the bypass loads (tension or compression), the diameter D of the fasteners and the loading direction. Moreover, the hole coefficient also depends on the pitch w, and whether it is large enough for the holes to be considered independent or not (w < 5D). Figure 5 : Multilevel strategy to study the failure of a complex joint structure. In our point of view, the industrial strategy to predict the failure of complex joint is very efficient in a modeling point of view. Indeed, the computational cost are reduced thanks to the multilevel strategy. However, the main drawback of this method lies in the identification of the parameters K t and K m which necessitates a huge experimental database. This is the reason why we propose in this paper a virtual testing strategy to identify this parameter (right of Figure 5).
9 Application of the virtual testing strategy to an industrial case The present virtual testing strategy is applied in the section to an industrial test case presented in Figure 6. It is a generic bolted joint structures composed of three omposite panels and light alloy buttstraps. The study is focused on panel 1 [0/45/0/45 /0/ 45 /0/45/0 3 /45/90/45/0 /45/0 /45/90] s. manufactured using T700/M1 unidirectional plies. The structure is subjected to a shear test in a doubleframe device (see mesh and boundary conditions in Figure 6b). (a) (b) Figure 6 : Picture of the composite junction subjected to a doubleframe shear test (a) FE mesh and detail of the structure (b). The identification of parameters K t and K m has necessitate to perform FE calculation, using the model presented in the first section, for (i) openhole test, (ii) bearing tests and (iii) plane plate specimen with the nominal layup disoriented with an angle varying form 0 to90. Fifteen virtual tests have been necessary to identify these parameters. Finally, this analysis permit to perdict a failure load equal to 1390kN to be compared with the experimental load equal to 160kN. The error is lower than 10%. CONCLUSION This study was aimed at proposing tools to increase the complexity and decrease the calculation cost for strength prediction of bolted junctions. This approach is based on a classical industrial multilevel strategy. A global calculation is first performed in order to evaluate the behaviour of the whole junction in its environment. The strength of the critical fixations is, in a second time, evaluated at locallevel calculations. This local analysis is based on a simple semiempirical model industrially identified on a huge experimental data basis. In order to reduce this experimental cost, a virtual testing approach is proposed. The virtual tests use a detailed simulation, physically based but very time consuming. This fine model permits reproduce the experimental results for various loading (openhole and filledhole in tension, joints subjected to combined bybass and bearing load). It has been shown that such a virtual testing strategy has permit predict to failure load of a complex bolted joint structure.
10 ACKNOWLEDGEMENTS This work was carried out under the AMERICO project (Multiscale Analyses: Innovating Research for Composites) directed by ONERA and funded by the DGA/STTC (French Ministry of Defence) which is gratefully acknowledged. References 1. Aktas A., Dirikolu M.H., "An experimental and numerical investigation of strength characteristics of carbonepoxy pinnedjoint plates", Composites Science and Technology 64, pp , 004. Whitworth H.A., Aluko O., Tomlinson N.A., "Application of the point stress criterion to the failure of composite pinned joints", Engineering Fracture Machanics, 007, doi: / /j.engfracmech Camanho PP, Matthews FL. A progressive damage model for mechanically fastened joints in composite laminates. Journal of Composite Materials 33, 10, pp , McCarthy M.A., McCarthy C.T., Lawlor V.P., Stanley W.F., "Threedimensional finite element analysis of singlebolt, singlelap composite bolted joints: Part I  model development and validation", Composite Structures 71, pp , Koerber H., Camanho P.P., Simulation of Progressive Damage in Bolted Composite Joints, Proceedings of the 13 th European Conference on Composite Materials, June 5, 008, Stockholm, Sweden 6. Dano M.L, Gendron G, Picard A., "Stress and failure analysis of mechanically fastened joints in composite laminates", Composite Structures 50, pp , Laurin F., Carrere N., Maire J.F., "A multiscale progressive failure approach for composite laminates based on thermodynamical viscoelastic and damage models", Composite Part A, 38, pp , Allix O., Deü J.F., Ladevèze P., "A delay damage mesomodel for prediction of localisation and fracture of laminates subjected to high rates loading". ECCM'99, Munich, Tvergaard V., "Effect of fibre debonding in a whiskerreinforced metal", Materials Science and Engineering, pp , Irisarri F.X, Strategie de calcul pour l optimisation multiobjectif des structures composites, PhD Thesis, Université Toulouse III, Toulouse, France, Ekh J., Schön J., "Load transfer in multirow, single shear, compositetoaluminum lap joints", Composites Science and Technology 66, pp , Sardin J., Rapport d'essai n M06/698000/P1/A, PEA Americo Tranche 4, Centre d'essais Aéronautique de Toulouse, 007
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More informationCohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
University of Liège Aerospace & Mechanical Engineering Cohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationTOWARD VIRTUAL CERAMIC COMPOSITES
TOWARD VIRTUAL CERAMIC COMPOSITES M. Genet 1, P. Ladevèze 12, G. Lubineau 1 1 LMTCachan (ENSCachan, CNRS, Paris 6 University, UniverSud Paris PRES) 61 avenue du Président Wilson 94235 Cachan CEDEX {genet,
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationFRACTURE MECHANICS IN ANSYS R16. Session 04 Fracture Mechanics using Cohesive Zone Material (CZM) Model
FRACTURE MECHANICS IN ANSYS R16 Session 04 Fracture Mechanics using Cohesive Zone Material (CZM) Model COHESIVE ZONE MATERIAL MODEL (CZM) Fracture or delamination along an interface between phases plays
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationDamage analysis of composite structures: a software editor point of view and illustration on industrial applications
1 SAMCEF Solver group, SAMTECH s.a., A Siemens Company 2 Aerospace & Mechanical Engineering Dpt, University of Liège Damage analysis of composite structures: a software editor point of view and illustration
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationAnálisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas
San Miguel de Tucuman, Argentina September 14 th, 2011 Seminary on Análisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas Antonio Caggiano 1, Guillermo Etse 2, Enzo
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationSIMULATION OF BOND FAILURE IN RC BEAMS STRENGTHENED WITH FRP SHEETS SUBJECTED TO DYNAMIC/IMPACT LOADINGS
Proceedings of International Symposium on Bond Behaviour of FRP in Structures (BBFS 005) Chen and Teng (eds) 005 International Institute for FRP in Construction SIMULATION OF BOND FAILURE IN RC BEAMS STRENGTHENED
More informationDELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE
DELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE F. LACHAUD 1,2, R. PIQUET 2, L. MICHEL 1 2 LMT, IUT de énie Mécanique, 50, Chemin des Maraîchers, 31077 TOULOUSE
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationEVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES
EVALUATION OF DEBONDING ENERGY RELEASE RATE OF EXTERNALLY BONDED FRP SHEETS FOR REHABILITATION OF INFRASTRUCTURES Koji YAMAGUCHI 1, Isao KIMPARA 1, and Kazuro KAGEYAMA 1 1 Department of Environmental &
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationDebonding process in composites using BEM
Boundary Elements XXVII 331 Debonding process in composites using BEM P. Prochazka & M. Valek Czech Technical University, Prague, Czech Republic Abstract The paper deals with the debonding fibermatrix
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationTowards a multiscale analysis of delamination in dynamics
ECCM 2010 Towards a multiscale analysis of delamination in dynamics Chloé DupleixCouderc (1), (2), Olivier Allix (1), Fabrice Gatuingt (1), Benoît Malherbe (2) (1) LMTCachan (ENS Cachan/CNRS/Université
More informationDAMAGE MODELLING OF A SATIN SEPCARB COMPOSITE
DAMAGE MODELLING OF A SATIN SEPCARB COMPOSITE X. Aubard 1, C. Cluzel 2,3, P. Ladevèze 2 and J.N. Périé 2 1 SEP Division de SNECMA, Le Haillan BP 37, 33165 St MEDARDENJALLES, FRANCE 2 LMT Cachan, E.N.S.
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationVIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS. Ana Andreia Pinheiro Durão Branco. Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho
VIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS Ana Andreia Pinheiro Durão Branco Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho Mestrado Integrado em Engenharia Mecânica July 17, 2015
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationNumerical modelling of contact for low velocity impact damage in composite laminates J. Bonini, F. Collombet, J.L. Lataillade
Numerical modelling of contact for low velocity impact damage in composite laminates J. Bonini, F. Collombet, J.L. Lataillade Esplanade des Arts et Metiers, INTRODUCTION A low velocity impact on a composite
More informationHEALTH MONITORING OF COMPOSITE STRUCTURES USING ULTRASONIC GUIDED WAVES
HEALTH MONITORING OF COMPOSITE STRUCTURES USING ULTRASONIC GUIDED WAVES P. BRASSIER, P. PERES, ASTRIUM SPACE Transportation, Avenue du Général Niox, BP 11, 33165 StMédardenJalles, FRANCE B. HOSTEN,
More informationMicromechanics of recycled composites
Monday, 21 st August 2011 Micromechanics of recycled composites for material optimisation and ecodesign Soraia Pimenta soraia.pimenta07@imperial.ac.uk S T Pinho, P Robinson Motivation Introduction recycled
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationFHWA Bridge Design Guidance No. 1 Revision Date: July 21, Load Rating Evaluation of Gusset Plates in Truss Bridges
FHWA Bridge Design Guidance No. 1 Revision Date: July 21, 2008 Load Rating Evaluation of Gusset Plates in Truss Bridges By Firas I. Sheikh Ibrahim, PhD, PE Part B Gusset Plate Resistance in Accordance
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationComposite Materials. FibreMatrix Interfaces. There is nothing there really except the two of you (or the fiber and matrix).
Composite Materials FibreMatrix Interfaces There is nothing there really except the two of you (or the fiber and matrix). Composite Parameters Fibre properties Composite Interfaces Matrix properties Fibre
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationDelamination in fractured laminated glass
Delamination in fractured laminated glass Caroline BUTCHART*, Mauro OVEREND a * Department of Engineering, University of Cambridge Trumpington Street, Cambridge, CB2 1PZ, UK cvb25@cam.ac.uk a Department
More informationCentrifuge Shaking Table Tests and FEM Analyses of RC Pile Foundation and Underground Structure
Centrifuge Shaking Table s and FEM Analyses of RC Pile Foundation and Underground Structure Kenji Yonezawa Obayashi Corporation, Tokyo, Japan. Takuya Anabuki Obayashi Corporation, Tokyo, Japan. Shunichi
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationAcoustic emission analysis for failure identification in composite materials
Acoustic emission analysis for failure identification in composite materials Markus G. R. Sause Experimental Physics II Institute of Physics University of Augsburg 1. Motivation 2. Methods of AE analysis
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationNumerical Vibration Analysis of Impacted CFRP Specimens Using COMSOL Multiphysics
Numerical Vibration Analysis of Impacted CFRP Specimens Using COMSOL Multiphysics Philipp Jatzlau 1, Florian Seybold 1 1 Technical University of Munich, Center for Building Materials, Chair of Nondestructive
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationFREE EDGE DELAMINATION ONSET CRITERION
FREE EGE ELAMINATION ONSET CRITERION G. MARION now, 2, formerl 3, R. HARRY 2, and F. LECUYER MEYSYS, 29 rue J. Rostand, 9873 ORSAY CEEX, FRANCE 2 Laboratoire de Génie Mécanique, IUT Bordeaux I, 3345 TALENCE
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationAnalysis and Optimization of a Hybrid Fan Blade
Analysis and Optimization of a Hybrid Fan Blade Permas Users Conference 27.04.06 28.04.06 Strassbourg DLR German Aerospace Center, Stuttgart Institute of Structures and Design J. Ehrmanntraut, F. Kocian,
More information